View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
Ashish Kumar Parashar, Rinku Parashar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1232-1236 The Effect of Size of Fibres on Compressive Strength of M-20 Concrete Mix Ashish Kumar Parashar*, Rinku Parashar** *Department of Civil Engineering, IT,GGV [Central University], Bilaspur, India ** Department of Architecture, National Institute of Technology, Raipur, IndiaABSTRACT bicycle (shown in Figure 1.1) are cut in particular The present scenario highlights the sizes for using as steel fibre. A total of 99 numbersdepleting non renueable resources, followed by a of concrete cube specimens were casted with anddrastic escalation in the cost of building without fibres and were tested under compression asmaterials. With the population explosion also the per relevant Indian standard specifications. Testconstruction activity is in its boom, resulting in result indicated that addition of steel fibres fromvariety of buildings being constructed globally. lathe increased the strength and many otherAs we all know concrete is one of the most properties of concrete but only up to certain limit ofimportant and versatile material playing an percentage.important role in the construction industry,being recognized world -wide. So an effort hasbeen made in this research to make a concretemix using, waste cycle spokes as reinforcement soas to make it easily available to the general publicat a reduced cost for specified type ofconstruction works, depending upon its strengthrequirement. Different type of concrete mix wasproportioned with varying quantity of Ordinary Figure 1.2 After CuttingPortland Cement and steel fibres and studied.The result depicted the variations in concrete 1.1 CONCRETE MIX DESIGNstrength with the gradual increase in the long The Concrete mix design can be defined assteel fibres. The present research work highlights the art of obtaining a concrete of the requiredas to how the compressive strength of the properties, at the lowest cost, by suitable choice andconcrete can be increased thus increasing its proportions, of available materials. Needless to say,strength and durability. a property designed concrete mix for the specified strength requirements should have the minimumKeywords - Concrete, Steel Fibres, Cycle spokes, cement content to make mix economical. It should,Strength, Steel Fibres Size, Durability, Economy however, be stressed that the precise relationship falls between the properties of concrete and the1. INTRODUCTION specific characteristics such as water cement ratio, Concrete is the most important construction aggregate cement ratio and grading, apart from suchmaterial, which is manufactured at site. Concrete elusive quantities as aggregate-particle shape andrequired for extensive construction activity can texture. Hence, concrete mix design cannot bealways be made available since all the ingredients of mechanically done and is likely to remain an art,concrete are materials of geological origin. Various rather than a science, for some time to come. Theresearch and effort have been made to obtain a purpose of concrete mix design is to ensure the mostdurable, strong and economical concrete mix. optimum properties of the constituent materials to meet the requirements of the structure being built. Mix design should ensure that the concrete: Complies with the specifications of structural strength laid down, which is usually stated in terms of the compressive strength of standard test specimens. Complies with the durability requirements to resist the environment in which the structure will serve its functional life. Be capable ofFigure1.1 Bicycle Spokes being mixed, transported, and compacted asThe investigation reported in present work was efficiently as possible without undue labour. Andcarried out to study the feasibility of using waste last, but not least, be as economical as possible. Thesteel fibres in two different sizes viz. 30 mm and 50 design of concrete is science that can be describedmm in fibre reinforced concrete. Waste Spokes of 1232 | P a g e
Ashish Kumar Parashar, Rinku Parashar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1232-1236here only in its broad outlines. The starting point of testing, the study of aggregates has been doneany mix design is to establish the desired under the following subheadings:workability characteristics of wet concrete, the Sizedesire physical properties of the cured concrete and Specific Gravitythe acceptable cost of the concrete. Moisture Content Sieve Analysis2. MATERIALS USED FOR MIX DESIGN Grading2.1 AGGREGATE The aggregate is the matrix or principal 2.2.3 SIZEstructure consisting of relatively inert fine and The largest maximum size of aggregatecoarse material. The aggregate for concrete varies in practicable to handle under a given set ofsizes, but in any mix the particles of different sizes condition should be used. Using the largestare used. The particles size distribution is called the possible maximum size will result in:grading of the aggregate. While producing good Reduction of cement contentquality concrete the aggregate is used at least from Reduction in water requirementtwo size groups. Reduction of drying shrinkage However, the maximum size of aggregate2.1.2 FINE AGGREGATE that can be used in any given condition may be IS:-383-1963 destines the fine aggregate as limited by the following condition:the aggregate which will pass through 4.75 mm IS Thickness of sectionsieve. The fine aggregate is often termed a sand size Spacing of reinforcementaggregate. Clear cover Mixing, handling and placing techniques2.2.2 COARSE AGGREGATE Generally, the maximum size of aggregate Coarse aggregate shall consist of crushed should be as large as possible within limitsor broken stone and be hard, strong, dense, durable, specified, but in any case not greater than one-clean or proper gradation and free from skin and fourth of the minimum thickness of the membercoating likely to prevent proper adhesion of mortar. provided.The aggregate shall generally be cubical in shape asfar as possible flaky, elongated pieces shall be 2.2.4 SPECIFIC GRAVITYavoided. Unless special stone of particular quarries Specific gravity of aggregate is made useare mentioned in the special provisions, aggregate of, in design calculations of concrete mix. Withshall be broken from the best the specific gravity of each constituent known, itstrap/granite/quartzite/geness stones in that order weight can be converted into solid volume andavailable in the region and approved by the hence a theoretical yield of concrete per unitEngineer. volume can be calculated. Average specific The maximum size may be up to 80 mm gravity of the rock varies from 2.6 to 2.8.and well graded between the size 5mm to 80mm insuch proportion as to give maximum density to the 2.2.5 MOISTURE CONTENTconcrete. The maximum size should be as large as Some of the aggregate are porouspossible within the above limit but should not and absorptive. Porosity and absorption ofexceed 1/4 of minimum thickness of the member aggregate will affect the water cement ratio andprovided. However, this size presents no difficulty the workability of concrete and sometimes alsoin the case of R.C.C. to surround the reinforcement affect the durability of concrete.thoroughly and fill up the corners of the formworksatisfactorily. 2.2.6 SIEVE ANALYSIS In the case of general concrete work, Sieve analysis is the name to themaximum size of 40 mm is used and in R.C.C. work operation of dividing a sample of aggregate intoa maximum size of 20 mm (about 3/4) will be found various fraction each consisting of particles of thesatisfactory but it should be restricted to 6 mm same size. The sieve analysis is conducted to(about 1/4) less than the minimum lateral cleat determine the particle size distribution in sampledistance between bars or 6 mm (about11/4) less than of aggregate, which is called gradation. In thisthe cover whichever is smaller. The crushing connection a term known as “Fineness Modulus”strength of aggregate will be such, as to allow the is being used. The fineness modulus is aconcrete in which it is used to build up the specified numerical index of fineness, giving some ideas ofstrength of concrete. the mean size of the particles present in the entire To know more about the concrete it is very body of the aggregate. Hard and bitter wateressential that one should know about aggregate, containing more than p.p.m. of sulphates shall notwhich constitute major volume in concrete. For be used for curing purpose. Probable water 1233 | P a g e
Ashish Kumar Parashar, Rinku Parashar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1232-1236 generally is found suitable for curing cement Steel fibers are made of cold drawn steel concrete. wire with low content of carbon (C) or stainless steel wire (SS 302/ SS 304). Steel fibers are Type of sand Fineness Modulus manufactured in different types: hooked, undulated Fine sand 2.2 - 2.6 or flat, according to the construction project. These fibers are used in construction, for concrete Medium sand 2.6 - 2.9 reinforcement. Coarse sand 2.9 - 126.96.36.199 GRADATION The particle size distribution of anaggregate as determined by sieve analysis is termedas grading of aggregate. The grading of aggregate isexpressed in terms of percentage by weight, retainedon or passing through a series taken in order, 80mm,40mm, 20mm, 10mm, 4.75mm, for coarse aggregateand 10mm, 4.75mm, 2.36mm, 1.18mm, 600 Figure 4.1.1 - Types of Steel Fibersmicrons, 300microns, for fine aggregate. Thegrading of aggregate affects the workability, whichin turn, controls the water and cement requirements,segregation and influences the placing and finishingof concrete. There is no universal ideal gradingcurve. However, IS:383-1970 has recommendedcertain limits within which the grading must lie toproduce satisfactory concrete, subjected to thefulfillment of certain desirable properties of Figure 4.1.2 – Types of Steel Fibresaggregate, such as shape, surface texture, type ofaggregate and amount of flaky and elongated Fiber-reinforcement is mainly used inmaterials. shotcrete, but can also be used in normal concrete fiber; Steel fibers reinforced concrete are less3. PROPERTIES OF FRESH CONCRETE expensive than hand-tied rebar, while still Fresh concrete is a mixed material, which increasing the tensile strength many times; Shape,can be, moulded into any shape. The relative dimension and length of fiber are important Aquantities of cement, aggregate and water mixed normal size fibre is 30 to 60 mm. Steel fibers cantogether control the properties of concrete in the wet only be used on surfaces that can tolerate or avoidset state as well as in the dry state. It depends upon corrosion and rust stainsthe water cement ratio and the workability of 4.2 SHAPES AND SIZES OF STEEL FIBRESconcrete.3.1.1 Water for mixing cement concrete Water for mixing cement concrete shall not besalty or brackish but shall be clean/reasonably clear,free from objectionable quantities of silt and tracesof oil, acid and injurious alkali, salts, organic matterand other such materials which will either weaken Figure 4.2[a] Figure 4.2 [b]the mortar or cement or cause efflorescence orattack steel in R.C.C. Water should be maintained insuch a manner so as to exclude silt, mud, grass orother foreign materials. Containers for transport,storage and handling of water shall be clean. Waterfit for drinking shall generally be found suitable formixing cement/lime concrete or mortar.3.1.2 Curing cement concrete Figure 4.2 [c] Figure 4.2 [d] Water for curing mortar or concrete shouldnot be too acidic or too alkaline. It shall be free of Steel Fibres are available in different shapeelement, which significantly affect the hydration and size. Figure 4.2 [a,b,c,d] shows different typereaction or otherwise interfere with the hardening. of steel fibres.4. STEEL FIBRES FOR CONCRETE REINFORCEMENT 1234 | P a g e
Ashish Kumar Parashar, Rinku Parashar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1232-12365. LABORATORY TEST & COMP. STRENGTH OBSERVATIONS 30 OPC The total 99 numbers of concrete cube 25 20 (N/mm2)specimens were casted with using waste steel fibres(bicycle Spokes). Cubes of without fibres and with 15 10 FRCfibres were tested under compression as per relevant 5 30Indian standard specifications Comparative Test 0results in figures were represented below: mm 3 7 28 Age (Days) 30 OPC COMP. STRENGTH 25 Figure- 5.4 Comparison of Average Comp. 20 Strength of Concrete Mix [M-20] made by using FRC 30 (N/mm2) 15 OPC, and OPC with 20% Steel Fibres 10 mm 5 FRC 50 COMP. STRENGTH OPC 0 mm 30 25 3 7 28 (N/mm2) 20 FRC 30 Age (Days) 15 10 mm 5 0 FRC 50 mmFigure- 5.1 Comparison of Average Comp. 3 7 28Strength Age (Days) of Concrete Mix [M-20] made by using OPC, and OPC with 5% Steel Fibres Figure- 5.5 Comparison of Average Comp. Strength of Concrete Mix [M-20] made by using OPC, and OPC with 25% Steel Fibres COMP. STRENGTH 30 30 25 OPC 25 20 (N/mm2) 20 15 FRC 15 10 30 mm 10 5 FRC 5 0 0 50 mm 3 7 28 3 days 7 days 28 days Age (Days) OPC 5 % FRC 10 % FRC 15 % FRC 20 % FRC 25 % FRC Figure- 5.6 (a) Comparison of Average Comp.Figure- 5.2 Comparison of Average Comp. Strength of Concrete Mix [M-20] made byStrength of Concrete Mix [M-20] made by using using OPC, and 30 mm size Steel Fibres with OPC, and OPC with 10% Steel Fibres different % 30 25 30 20 OPC 15 COMP. STRENGTH 25 10 20 5 FRC 30 15 (N/mm2) mm 0 10 FRC 50 3 days 7 days 28 days 5 mm OPC 5 % FRC 10 % FRC 0 15 % FRC 20 % FRC 25 % FRC 3 7 28 Age (Days) Figure- 5.6 (b) Comparison of Average Comp.Figure- 5.3 Comparison of Average Comp. Strength of Concrete Mix [M-20] made by usingStrength of Concrete Mix [M-20] made by using OPC, and 50 mm size Steel Fibres with differentOPC, and OPC with 15% Steel Fibres % 1235 | P a g e
Ashish Kumar Parashar, Rinku Parashar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1232-1236 curing. When 20%, 25% of 30 mm long Steel Fibre by weight was allowed to mix in OPC for making concrete its strength increased for 7 days and 28 days as compared to plain cement concrete represented by Figures- 5.4 & 5.5. When 15%, 20% & 25% of 50 mm long Steel Fibre by weight was allowed to mix with OPC for making concrete its strength also increased for 7 (a) (b) days and 28 days as compared to plain cement Figure 5.7 – 30MM Fibres (a) & 50MM Fibres concrete. (b) used for Concrete Mix [M-20] Thus from above study it was concluded that the 28 days compressive strength of concrete mixed (M20), containing Steel Fibre in varying percentage of steel Fibre (viz. 5% & 10%) was slightly less than the strength of Plain Cement Concrete. But it was possible to increase other properties of concrete like durability, cracking resistance, fire resistance property etc. The present study showed that compressive strength increased when we allow more than 10 % with size 30mm & 50mm long Figure 5.8 –Mixing of Fibres Steel Fibres were used. The present study indicates that to increase compressive strength of concrete when the steel fiber from bicycle spokes were used. For making higher strength at nominal mix proportion by allowing 25%, 50 mm long Steel Fibre in Plain M- M-20 grade of concrete & save the cement quantity. For different concrete structural works we hope that present study will act as guidance for the fiber use in concrete for strength, durability and economy. Figure 5.9 –Cube Test of Fibres Mixed Concrete References6. CONCLUSIONS  Arnon Bentur & Sidney Mindess, „„ Fibre The aim of Mix Design was to make a reinforced cementitious composites‟‟ Elsevier applied science London and Newyork 1990.concrete of desirable strength, durability and  Colin D. Johnston, “Fiber reinforced cements andeconomy. The present study reveled the effect of concretes” Advances in concrete technologysize of fibres on compressive strength of M-20 volume 3 – Gordon and Breach Science publishesconcrete mix design. The waste product “steel fiber – 2001.from bicycle spokes” were mixed as ingredients of  C.H. Henager , “Steel fibrous shotcrete”. Aconcrete and were studied in terms of strength of summary of the State – of – the art concrete Int.:concrete and following results were obtained- Design and construction 1981.Figure- 5.1 shows that when 5% of 30 mm & 50  C.D. Johnston, “Steel fiber reinforced mortar andmm long Steel Fibre by weight were allowed to mix concrete”, A review of mechanical properties. In fiber reinforced concrete ACI – SP 44 – Detroitwith OPC for making concrete, its strength 1974.increased up to 7 days as compared to plain cement  JCI Standards for Test Methods of Fibre Reinforcedconcrete and then strength decreased after 28 days Concrete, Method of Test for Flexural Strengthcuring. and Flexural Toughness of Fibre ReinforcedWhen 10% of 30 mm & 50 mm long Steel Fibre by Concrete (Standard SF4), Japan Concrete Institute,weight was allowed to mix on OPC for making 1983, pp. 45 – 51.concrete, its strength increased up to 7 days as  J. Endgington, D.J. Hannant & R.I.T. Williams,compared to plain cement concrete but strength “Steel fiber reinforced concrete” Current paper CPincreased only in 30 mm long Fibre and strength 69/74 Building research establishment Garston Watford 1974.decreased when 50 mm long Fibre were used for 28  Perumalsamy N. Balaguru, Sarendra P. Shah,days of curing represented by Figure- 5.2. „„Fiber reinforced cement composites‟‟ , Mc GrawFigure- 5.3 shows that when 15% of 30 mm & 50 Hill International Editions 1992.mm long Steel Fibre by weight was allowed to mix  R.J. Craig, “Structural applications of reinforcedwith OPC for making concrete, its strength steel fibrous concrete”. Concrete Int. Design andincreased up to 7 days as compared plain cement Construction 1984.concrete and also strength increased after 28 days 1236 | P a g e